Corrosion engineering FAQ

corrosion in stainless

The pitting resistance of stainless steel is primarily determined by its composition. The three elements which have a significant beneficial effect are chromium, molybdenum, and nitrogen. The formula which gives their relative contribution is:

PREN=%chromium+3.3x%molybdenum+(16 to 30)x%nitrogen, where PREN is pitting resistance equivalent number and percents are in weight percent of elements IN SOLID SOLUTION. Ferritic stainless steels, which can hold no nitrogen in solid solution, must obtain all their corrosion resistance from chromium and molybdenum. The nickel in austenitic stainless steel confers no benefit; it only stabilizes the austenitic structure, which can hold appreciable nitrogen.

Recent research has shown that pitting susceptibility arises from the bulk material around the manganese sulfide inclusions losing chromium as sulfur precipitates as chrome sulfide around the pre-existing primary manganese sulfide inclusion. This occurs during cooling from melting temperatures. This region can have less than 10% chrome. Thus, it corrodes away as would carbon steel, initiating the pitting process. The inclusion itself is not the initiator of pitting.Welds (GTAW or TIG)have significantly lower pitting resistance. Their PREN is reduced by 335x(%S) and 700 to 1000 x (%O). These elements form chromium bearing inclusions during weld cooling and deplete the surrounding matrix of chromium. Removing oxides from welds is important, but so is removing the chromium depleted regions by pickling and passivating.

My Archive

Resources

ENGINEERING.com surveyed 364 product development professionals to glean insights into how their teams are performing today, and what technologies are most useful to support their processes. Download Now

3D printing has quickly expanded beyond the realm of prototyping and into the world of end part manufacturing. Desktop 3D printers need not be used for making parts themselves, but as a secondary process for producing tools. Download Now

Creating tooling for injection molding is an expensive and complex proposition. Until recently, the only way to avoid tooling defects causing air traps, voids, shrinkage and the like was to employ a time-consuming and tedious physical prototyping process. Download Now